Tips & Tricks
Like this document? Why not share!
Email sent successfully!
Show related SlideShares at end
May 23, 2014
Comment goes here.
12 hours ago
Are you sure you want to
Your message goes here
Be the first to comment
Be the first to like this
Number of Embeds
No notes for slide
Transcript of "40120140505001"
1. International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 1 CHARACTERIZATION AND PROPERTIES EVALUATION OF CONDUCTING Al - DOPED ZnO AT LOW TEMPERATURE BY ECD METHOD Harish Chevva1 , Sanjay.S2* 1 Centre for Nanotechnology Research, VIT University, Vellore, Tamil Nadu, India 2* Dept. of Biomedical Engineering, Bharath University, Chennai, Tamil Nadu, India ABSTRACT Low temperature (70˚C) deposition of Al-doped ZnO films are successfully reported by simple electrochemical deposition technique. Simple three electrode setup is used with chemical bath containing different molar ratios of Zinc nitrate and Aluminium nitrate (9:1, 8:2, 7:3 and 6:4), a constant potential of -1.3 V is employed between electrodes for deposition of films. ‘2θ’ and ‘d’ spacing variations obtained from XRD with varied Al content proves doping of Al into crystal structure of ZnO. Al content from Elemental analysis (EDAX) is in accordance with the compositions used. Morphology of films is characterized by FE-SEM, where flake-like structures are observed. Variation of Electrical resistivity with varying Al content in the films supports the argument of doping. Lowest resistivity is observed for composition 7:3 i.e. 2.25x10-4 cm. Optical characterization is done on the film powder for measuring band gap and transmittance, which showed 90% of transmittance and Band gap widening is observed for different compositions, due to incorporation of Al into crystal structure of ZnO. Keywords: Electrochemical, ZnO, Al Doped, XRD Band Gap Widening and Transmittance. 1. INTRODUCTION Zinc oxide is an N – type semiconductor which is having wide band gap of ~3.3 eV. ZnO mainly exists in two crystalline structures hexagonal Wurtzite and cubic Zincblende, wurtzite is most common structure found because of its formation at room temperature conditions. The growing interest in research on ZnO in recent days is on account of its special properties like Tunable band gap, transparent nature and UV light sensing. Some of the devices that are built by ZnO thin films are Nano – floating gate devices , UV sensors , Pizeo electric devices, Antireflective coatings , Gas sensor  and solar cell . INTERNATIONAL JOURNAL OF ELECTRONICS AND COMMUNICATION ENGINEERING & TECHNOLOGY (IJECET) ISSN 0976 – 6464(Print) ISSN 0976 – 6472(Online) Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME: www.iaeme.com/ijecet.asp Journal Impact Factor (2014): 7.2836 (Calculated by GISI) www.jifactor.com IJECET © I A E M E
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 2 Doping of ZnO is carried out in order to improve the properties of ZnO like transparency and conductivity. Wide variety dopant materials are available, which are successfully incorporated into the crystal structure of ZnO. Depending on the change in property of ZnO by adding dopant, doping is classified into two n-type and p-type. Some of dopants reported till now as dopants to ZnO structure are Gallium [4, 6], Erbium , Aluminum [3, 5, 7 - 11], Gold , Cobalt , Vanadium , Yttrium , Silver , Copper , Tin , Palladium , Cerium , Nickel , Iron , Manganese [22, 23], Magnesium , Lithium  and Nitrogen . Among all the above dopants, Al is most used dopant because of its nature to enhance some properties of ZnO like enhancement of Band gap, transparency, electrical conductivity and nontoxicity. There are many techniques employed for doping of Al like RF sputtering , Vacuum metal deposition (VMD) , RF Magnetron Sputtering [29, 32, 34], Reactive sputtering process , MOCVD , Sol gel process [33, 38], Pulsed electron deposition , DC Magnetron sputtering , Spray – Pyrolysis . There are many other methods which are mentioned above which can incorporate Al into crystal structure of ZnO, and have obtained promising results in terms of Electrical resistivity and Optical transmission, but all these methods need large equipment, heavy maintenance, high power and other parameters like pressure, voltage etc. so there is need for simple method that can successfully incorporate Al into crystal structure of ZnO. Our method employed here is very simple, low temperature deposition technique, takes less time of deposition and can be employed for larger area coatings easily. Comparison of results obtained by other methods and remarks on its operations is listed in below Table.1. Table 1: Comparison of results obtained by other methods of Al doping Deposition method Electrical Conductivity Optical Properties Remarks RF Sputtering  6 x 10-4 cm 85% (Transmittance) Use of Hydrogen gas while deposition and high temperatures of 100 - 250˚ C Reactive Sputtering Process  1.43 x 10-3 cm 90.5 % Use of high base pressure and employing H2/(Ar + H2) RF Magnetron Sputtering  4.8 /sq 85% High power of 120W and temperature of 300˚ C MOCVD  1.9 cm 80% High temperature of 620˚C and use of CO2 gas PED  3.4 x 10-2 cm 80% High discharge voltage of 20kV In comparison to above methods, solution processing using Electro deposition technique is low temperature, very simple method and can obtain large area deposition. There are many reports regarding deposition of pure and doped ZnO using electro deposition such as Indium, cobalt and Nickel [39-51], Al reacts fast with oxygen to form Aluminum hydroxide when it is used in solution processing method like electro deposition, so they are very less reports on Al doping of ZnO using electro deposition. By varying parameters such as distance between electrodes, temperature of
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 3 electrolyte used and voltage of deposition, we can avoid the formation of secondary phase of Al and instead incorporate Al into crystal structure of ZnO. In this paper we are reporting successful doping of Al in to crystal structure of ZnO by verifying the same from XRD peaks which showed no secondary phase formation, EDAX which is in accordance with zinc nitrate and Aluminum nitrate compositions used. Electrical resistivity and optical band-gap measurements also support the doping of Al. 2. EXPERIMENTAL DETAILS 2.1 Deposition of Films Electro-deposition of Al doped ZnO films are carried out at temperature of 700 C by three electrodes configuration shown in fig 1, in which Ag/AgCl is used as reference electrode, Pt wire is used as counter electrode and Zn foil (0.5 cm2 ) is used as working electrode. Electrolyte used is mixture of source material as Zinc nitrate hexa hydrate (Zn (NO3)2 6H2O) and dopant material as Aluminum Nitrate (Al (NO3)2 9H2O) of different molar ratios of 9:1, 8:2, 7:3 and 6:4 respectively. Before deposition rigorous stirring is done for making dopant material completely dissolved in the electrolyte. Amperometric (i – t curve) technique is used for deposition of films with CH Instrument, at a constant voltage and time of -1.3 V and 15 min, respectively. The optimized distances between the electrodes for which we obtained continuous films were, distance between working and counter electrode is 1.5cm, working and reference electrode is 2cm and counter and reference electrode is 2.5cm. Fig 1: Schematic diagram of Electrochemical cell; W (working electrode-Zn foil), C (counter electrode-Pt wire) and R (reference electrode-Ag/AgCl) 2.2 Characterization details Crystal structure and phase changes due to doping were characterized by X-ray diffraction (XRD, D8 Advance, BRUKER, Germany, Cu-Kα: λ=0.1540598 nm). Surface morphology examined by FE-SEM () and elemental composition of doping element in the deposited films was obtained from EDAX. Resistivity measurements of the films are carried out by two point probe method. Surface height of film on the substrate is measured by using AFM (NanoSurf Easy Scan2, Switzerland). Absorption, Transmittance and Optical band gap curves of colloidal powder of films are obtained from Diffuse Reflectance UV-Vis spectrophotometer (JASCO V-670)
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 4 2.3 Resistivity Measurements Resistivity of deposited films is measured by two probe technique. Film Thickness is measured by AFM and obtained as ̴ 1.5 µ m. Resistivity is calculated using below formula. Resistivity (ρ) -cm = R*W*t/L (1) where ‘R’ is resistance obtained by two probes method, ‘W’ is contact width of probes, ‘t’ is thickness of the film and ‘L’ is distance between probes. 3. RESULTS AND DISCUSSION Figure 2 shows the XRD patterns of pure and doped ZnO films of different compositions mentioned. Predominant peaks (100), (002) and (101) are observed in the range of ‘2θ’ values of 31.56˚ to 35.84˚, which corresponds to hexagonal Wurtzite structure and there is no peak observed corresponding to secondary phase formation due to oxidization of Al. Lattice parameters of ‘a’= 3.282, ‘c’=5.26 and corresponding ‘c/a’ ratio of 1.602 closely matches with standard values of hexagonal structure. From the peaks, it can be observed that there is slight increase in the 2θ values, which corresponds to the decrease in ‘d’ spacing of respective planes. Table 1 shows corresponding ‘2θ’ and ‘d’ spacing values of pure and doped ZnO films. 20 30 40 50 60 0 3000 6000 9000 12000 Intensity(a.u.) 2 θθθθ (degrees) * * ZnO * Zn foil (100) (002) (101) (100) (101) (102) (102) (110) * Pure ZnO 9: 1 8: 2 7: 3 6: 4 Fig 2: XRD plots of Pure and Al doped ZnO compositions The increase in ‘2θ’ values and decrease in ‘d’ spacing values is due to incorporation of Al atom into crystal structure of ZnO, which can be in two ways: one is replacing Zn atoms and other is sitting in interstitial places of ZnO crystal structure. Al3+ ion in four coordination and has size of 54 pico meter which is less than size of Zn2+ ion size of 74 pico meter in the same coordination, which depicts that if Al replaces Zn atom in the structure, ‘d’ spacing of planes will decrease, which gives basic proof that Al is successfully doped into ZnO.
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 5 Table 2: Variation in ‘2θ’ and ‘d’ spacing values for different molar ratios From all the XRD plots, it is seen that (100) peak have high intensity which represents formation of flake-like structures of ZnO. Fig 3 shows an expanded view of XRD patterns showing only dominant peaks. From this figure, it is apparent that there is decrease in the intensity of peaks with increase in the content of Al, which could be due to decrease in the crystalinity of films . From Table 2 it is observed that for the 6:4 composition there is reverse trend, i.e. increase in ‘d’ spacing, which denotes that it is the saturation point of Al content for doping. 30 31 32 33 34 35 36 37 2000 4000 6000 8000 10000 Intensity(a.u.) 2θθθθ (degrees) PureZnO 6:4 7:3 8:2 9:1 Fig 3: XRD plots of dominant peaks of different molar compositions Fig 4 shows Morphology characterization using FE-SEM for all compositions obtained. Mostly flake like structures are seen corresponding to formation of ZnO structures, which is in line with the dominant (101) peak observed in XRD results. Molar compositions (Zn nitrate: Al nitrate) 2 Theta “d” spacing (100) (002) (100) (002) Pure ZnO 31.491 34.160 2.83859 2.62268 9:1 31.256 33.921 2.85944 2.75584 8:2 31.379 34.031 2.84853 2.63230 7:3 31.431 34.073 2.84391 2.62919 6:4 31.341 34.089 2.85190 2.62795
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 6 Fig 4: FE-SEM images of Al-doped ZnO films deposited using different molar compositions Elemental analysis (EDAX) is done to characterize the amount of Al content in the films deposited. Fig.5 shows the EDAX plots of all films of different compositions with contents of Al, O and Zn. Analysis is carried out at different regions of the films in order to obtain the minimum and maximum amounts of Al. Table 3 shows atomic percentage of Al, Oxygen and Zinc contents at different regions. Table 3: EDAX analysis data of Al, Zinc and oxygen contents with varying compositions Composition (Zinc nitrate: Aluminium nitrate) At% of Zn At% of O At% of Al Min Max Min Max Min Max 9: 1 62.61 79.30 19.22 36.23 1.16 2.38 8: 2 42.69 47.85 51.47 55.40 0.68 1.91 7: 3 40.52 40.53 56.46 57.17 2.3 3.02 6: 4 37.57 43.29 54.09 57.49 2.62 4.98
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 7 Fig 5: EDAX for different compositions films a) 9:1, b) 8:2, c) 7:3 and d) 6:4 Al content in films of different compositions closely matches with the respective composition used for deposition of films, which supports the argument of Al doping. Resistivity measurements of the films are done using simple two probes resistivity method. From all above discussions, we can draw basic conclusion that Al is doped into the crystal structure of ZnO. If it is the case Al3+ ions which replaced Zn2+ atoms initiate in the electron flow in the films which decreases resistivity of films. Fig.6 shows plot of resistivity values with variation in the content of Al. pure ZnO 9: 1 8: 2 7: 3 6: 4 0 5 10 15 20 25 30 35 40 45 Resistivity(10-4ΩΩΩΩ-cm) Compositions Fig 6: Resistivity plot of different films deposited using different molar compositions dc a b 0 200 400 600 800 1000 0 1000 2000 3000 4000 5000 Element At % O K 36.23 AlK 1.16 ZnK 62.61 Zn Zn Al O 0 200 400 600 800 1000 0 1000 2000 3000 4000 5000 Element At % O K 55.4 AlK 1.91 ZnK 42.69 Zn Zn Al O 0 200 400 600 800 1000 0 1000 2000 3000 4000 5000 Element At% OK 56.46 AlK 3.02 ZnK 40.52 O Al Zn Zn 0 200 400 600 800 1000 0 1000 2000 3000 4000 5000 Element At % OK 57.48 AlK 4.94 ZnK 37.57 Al Zn O
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 8 As Al content is increased, resistivity decreases, which is in line with above discussions of doping Al into the crystal structure of ZnO, lowest resistivity is obtain for 7:3 composition i.e. 2.25x10-4 cm. Increase in the resistivity for 6:4 composition is in accordance with the reversal of trends observed in XRD results, pointing to the saturation point of doping Al. All films are deposited on Zinc foil, so measurement of optical band gap and transmittance of the films is difficult, so the films are peeled off carefully from the substrate and are characterized by UV-VIS. Fig.7 (a) shows the plot of variation in the band gap for pure ZnO and 9:1 and 6:4 compositions films plotted using absorbance data of the powder and Fig.7 (b) shows the optical Transmittance of pure ZnO, 9:1 and 6:4 compositions. Fig.7: (a) (αhυ)2 Vs Photon energy (hυ) plots (b) Transmittance spectra for compositions pure ZnO, 9:1 and 6:4 compositions From Fig.7 (a) it can be observed that there is a band gap widening with the variation in Al content in the deposited films, this is due to the second argument discussed in XRD section the Al ions can also sit in interstitial places of ZnO structure which increase the band gap of of films. Transmittance plots plotted in the Fig.7 (b) shows the increase in the transmittance with doping which supports above discussion of band gap widening. Very good transmittance of 90% is obtained. From Transmittance graphs it can be seen that UV rays of wavelength below 300 can be blocked by using these films and as band gap engineering is possible with Al doping we can make use of these films for UV sensing devices. 4. CONCLUSION Successful doping of Al into crystal structure of ZnO and improvisation of electrical property and optical property of the deposited films by the increase of Al content is reported by just simple and low temperature deposition by three electrode electro deposition techniques. XRD and EDAX details support the above argument of Al doping. We obtained low resistivity of 2.25 * 10-4 for high doping composition of Al, obtained good optical transmission of 90% for doped ZnO which is more than that of pure ZnO. Optical band gap is also calculated using absorbance data and shows as there is as increase in composition of Al, the band gap is widening is observed. With all these results it can be concluded that deposited films show high conductivity, as well as high transmittance and with the opportunity of band gap engineering with varying Al content, these films will have potential usage in UV rays sensing devices. 300 400 500 600 700 800 10 20 30 40 50 60 70 80 Transmittance(%) Wavelength(nm) 9: 1 Pure ZnO 6: 4 3.0 3.1 3.2 3.3 3.4 0.3 0.6 0.9 1.2 1.5 hυυυυ (eV) (ααααhυυυυ) 2 (eV/cm) 2 Pure ZnO 9: 1 6: 4 a b
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 9 REFERENCES  Byoungjun Park, Kyoungah Cho, Sungsu Kim, Sangsig Kim Park et al.: Nanoscale Res Lett. 6, 41 (2011).  S.K. Panda, C. Jacob: Solid-State Electronics, 73, 44-50 (2012).  Bo-Yuan Su, Sheng-Yuan Chu, Yung-Der Juang, Mei-Chun Lin, Chia-Chiang Chang and Chin- Jyi Wu: J. Electrochem. Soc. 159, 312-6 (2012).  Moe Kevin, Wee Hong Tho and Ghim Wei Ho: J. Mater. Chem., 22, 1644 (2012).  H. Zhu, J. H¨upkes, E. Bunte, S.M. Huang S0169-4332(12)01368-2.  Erin L. Ratcliff, Ajaya K. Sigdel, Mariola R. Macech, Kenneth Nebesny, Paul A. Lee, David S. Ginley c, Neal R. Armstrong, Joseph J. Berry: Thin Solid Films, 520, 5652–63 (2012).  Ji-Zhou Kong Fei Zhou, Zheng Wang, Chuan-Bao Wang, Mei-Ling Wang, Kang-Min Chen, Xue-Mei Wu, Kong-Jun Zhu, Jin-Hao Qiu: J Sol-Gel Sci Technol, 63, 95–102 (2012).  Jianzi Li, Jian Xu, Qingbo Xu, Gang Fang: Journal of Alloys and Compounds, 542, 151–6 (2012).  R. Ebrahimifard, H. Abdizadeh, M. Reza Golobostanfard: Micro & Nano Letters, Received on 26th March 2012.  Byeong-Yun Oh, Jeong-Hwan Kim, Jin-Woo Han, Dae-Shik Seo a, Hwan Soo Jang, Ho-Jin Choi, Seong-Ho Baek, Jae Hyun Kim, Gi-Seok Heo, Tae-Won Kim, Kwang-Young Kim: Current Applied Physics, 12, 273-9 (2012).  T. Dimopoulos, G.Z. Radnoczi, Z.E. Horváth, H. Brückl: Thin Solid Films, 520, 5222–6 (2012).  N.L. Tarwal, R.S. Devan, Y.R. M, R.S. Patil, M.M. Karanjkard, P.S. Patil: Electrochimica Acta, 72, 32– 9 (2012).  Sesha Vempati, AmithaShetty, P.Dawson, KarunakarNanda, S.B.Krupanidhi: Journal of Crystal Growth, 343, 7–12 (2012).  J. ElGhoul, C. Barthou, L. ElMir: Physica, 44, 1910–5 (2012).  Necmettin Kılınç, Sadullah Öztürk, Lütfi Arda, Ahmet Altındal, Zafer Ziya Öztürk: Journal of Alloys and Compounds, 536, 138–144 (2012).  K. Thongsuriwong, P. Amornpitoksuk, S. Suwanboon: J Sol-Gel Sci Technol, 62, 304–12 (2012).  J. H. Zheng, J. L. Song, Q. Jiang, J. S. Lian: J Mater Sci Mater Electron, 23, 1521–6 (2012)  M. Vishwas, K. Narasimha Rao, K.V. Arjuna Gowda, R.P.S. Chakradhar: Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, 95, 423–6 (2012).  Jun bo Zhon, Jian zhang Li, Xi yang He, Jun Zeng, Yan Lu, Wei Hu, Kun Lin: Current Applied Physics, 12, 998-1001 (2012).  Mansoor Anbia, Seyyed Ebrahim Moosavi Fard: Journal of Rare Earths, 30, 38 (2012).  Shuangxue Zhao, Ping Li, Yu Wei: Powder Technology, 224, 390-4 (2012).  Yang Hailing, Xu Xiaoguang, Zhang Guoqing, Miao Jun, Zhang Xin, Wu Shizhe, And Jiang Yong: Rare Metals, 31, 154 (2012).  Cuong Ton-Thata, Matthew Foley, Matthew R. Phillips, Takuya Tsuzuki, Zoe Smith: Journal of Alloys and Compounds, 522, 114-7 (2012).  Qiang Shia, Junying Zhang, Dong Zhang, Changzheng Wanga, Bing Yang, Bingyuan Zhang, Wenjun Wang: Materials Science and Engineering B, 177, 689-693 (2012).  Pradipta K. Nayak, J. A. Caraveo-Frescas, Unnat. S. Bhansali, and H. N. Alshareef: Appl. Phys. Lett. 100, 253507 (2012).  Lingyun Zhanga, Yulin Yang, Ruiqing Fana, Haiyan Chen, Ruokun Jia, Yonghui Wang, Liqun M, Yazhen Wang: Materials Science and Engineering B, 177, 956-961 (2012).  X. Díez-Betriu, R. Jiménez-Rioboo, J. Sánchez- Marcos, E. Céspedes, A. Espinosa, A. de Andrés: Journal of Alloys and Compounds, (2012).  Meiqin Zhang, Gang Qin, Yueping Zuo, Ting Zhang, Yang Zhang, Lei Su, Hong Qiub, Xueji Zhang: Electrochimica Acta, 78, 412-6 (2012).  H.B. Zhou, H.Y. Zhang, Z.G. Wang, M.L. Tan: Materials Letters, 74, 96-9 (2012).
International Journal of Electronics and Communication Engineering & Technology (IJECET), ISSN 0976 – 6464(Print), ISSN 0976 – 6472(Online), Volume 5, Issue 5, May (2014), pp. 01-10 © IAEME 10  Naoki Tsukamoto, Nobuto Oka, Yuzo Shigesato: Thin Solid Films, 520, 3751-4 (2012).  Jianfeng Sua, Chunjuan Tang, Qiang Niu, Chunhe Zang, Yongsheng Zhang, Zhuxi Fu: Applied Surface Science, 258, 8595-8 (2012).  B.L. Zhu, J. Wang, S.J. Zhu, J. Wu, D.W. Zeng, C.S. Xie: Thin Solid Films, 520, 6963- 9 (2012).  Jianzi Li, Jian Xu, Qingbo Xu, Gang Fang: Journal of Alloys and Compounds, 542, 151-6 (2012).  N. Hirahara, Onwona-Agyeman, M. Nakao: Thin Solid Films, 520, 2123-7 (2012).  Pham Hong Quang, Ngo Dinh Sang, Do Quang Ngo: Thin Solid Films, 520, 6455–8 (2012).  Wonkyun Yang, Junghoon Joo: Current Applied Physics, 1, 5 (2012).  A. Crossay, S. Buecheler, L. Kranz, J. Perrenou, C.M. Fell, Y.E. Romanyuk, A.N. Tiwari: Solar EnergyMaterials&SolarCells, 101, 283-8 (2012).  Mingsong Wang, Weiqiang Liang, Yunfeng Yang, Juan Yang, Xiaonong Cheng, Sung Hong Hahn, Eui Jung Kim: Materials Chemistry and Physics, 134, 845-850 (2012).  Sanghwa Yoon, Ilgoo Huh, Jae-Hong Lim, Bongyoung Yoo: Current Applied Physics, 12, 784-8 (2012).  S. Kishwar, K. ul Hasan, N.H. Alvi, P. Klason, O. Nur, M. Willander: Superlattices and Microstructures, 49, 32-42 (2011).  O. Lupan, T. Pauporte, L. Chow, B. Viana, F. Pelle´, L.K. Ono, B. Roldan Cuenya, H. Heinrich: Applied Surface Science, 256, 1895-1907 (2010).  Bjoern Seipel, Athavan Nadarajah, Ben Wutzke, Rolf Könenkamp: Materials Letters, 63, 736-8 (2009).  Yiwen Tang, Lijuan Luo, Zhigang Chen, Yun Jiang, Bihui Li, Zhiyong Jia, Liang Xu: Electrochemistry Communications, 9, 289-292 (2007).  D. Ramırez, D. Silva, H. Gomez, G. Riveros, R.E. Marotti, E.A. Dalchiele: Solar Energy Materials & Solar Cells: 91, 1458-61 (2007).  E.A. Dalchiele, P. Giorgi, R.E. Marotti, F. Martın, J.R. Ramos-Barrado, R. Ayouci, D. Leinen: Solar Energy Materials & Solar Cells, 70, 245-254 (2001).  Chunfu Lin, Hong Lin, Jianbao Li, Xin Li: Journal of Alloys and Compounds, 462, 175-80 (2008).  J.S. Wellings, N.B. Chaure, S.N. Heavens, I.M. Dharmadas: Thin Solid Films, 516, 3893-8, (2008).  Hosang Ahn, Yaqi Wang, Seung Hyun Jee, Minseo Park, Young Soo Yoon, Dong-Joo Kim: Chemical Physics Letters, 511, 331-5 (2011).  Yi-Jing Li, Kun-Mu Li, Chiu-Yen Wang, Chung-I. Kuo, Lih-Juann Chen: Sensors and Actuators B, 161, 734-9 (2012).  B. Marı, F.J. Manjo´n, M. Mollar, J. Cembrero, R. Gomez: Applied Surface Science, 252, 2826-31 (2006).  Jaeyoung Lee, Yongsug Tak: Electrochemistry Communications, 22000 765–8 (2000).  M. Tortosa, F.J.Manjon, M.Mollar, B.Marı: Journal of Physics and Chemistry of Solids, 73, 1111-5 (2012).  Asish B. Mathews and Dr. Pavan Kumar Yadav, “Improved Linearization of Laser Source and Erbium Doped Fiber Amplifier in Radio Over Fiber System”, International Journal of Advanced Research in Engineering & Technology (IJARET), Volume 4, Issue 5, 2013, pp. 46 - 55, ISSN Print: 0976-6480, ISSN Online: 0976-6499.  A.S. Meena, P.L. Meena, M. Chandra, R. Meena, Shribai and R.C. Meena, “Electrochemical Studies of Anionic and Cationic Surfactants in Photogalvanic Cell for Solar Energy Conversion and Storage”, International Journal of Electrical Engineering & Technology (IJEET), Volume 4, Issue 4, 2013, pp. 180 - 187, ISSN Print : 0976-6545, ISSN Online: 0976-6553.  Prachi Sharma and Navneet Gupta, “Nanocrystalline Silicon Thin Film Transistor (Nc-Si:H Tfts)- A Device for Display Panels”, International Journal of Electronics and Communication Engineering & Technology (IJECET), Volume 4, Issue 7, 2013, pp. 115 - 127, ISSN Print: 0976- 6464, ISSN Online: 0976 –6472.